FORMATION OF SUPER SATURATED SOLID SOLUTION FE .peaks position as milling time increase and lead
Embed Size (px)
Transcript of FORMATION OF SUPER SATURATED SOLID SOLUTION FE .peaks position as milling time increase and lead
93 MS Proceedings of the 17th Int. AMME Conference, 19-21 April, 2016
17th International Conference on Applied Mechanics and Mechanical Engineering.
Military Technical College Kobry El-Kobbah,
FORMATION OF SUPER SATURATED SOLID SOLUTION FE-50WT.%CU BY HIGH ENERGY BALL MILLING (ATTRITOR)
A. E. Hannora*, F. F. Hanna and L. K. Marei
ABSTRACT High energy ball milling (attritor) was performed to synthesize Cu-50wt.% Fe super saturated solid solution at room temperature. The mechanically alloyed samples have been milled for 24 hrs and examined by X-ray diffraction (XRD) to investigate its microstructure. As a result of mechanical deformation a higher defect concentration generated in the powder and thus the crystallinity decreases as well as crystallite size. The magnetic properties assessments of as-milled samples were carried out using vibrating sample magnetometer (VSM).The magnetization decreases with milling time while the corecivity increases up to 12 hrs milling and then decreases.
KEY WARDS Fe-Cu, Mechanical milling, magnetic properties
Suez University, Faculty of Petroleum and Mining Engineering, Science and Mathematics Department, Suez, Egypt, 43721.
* Corresponding author's, Tel. +201147043930, Fax: +20623360252, E-Mail: firstname.lastname@example.org
94 MS Proceedings of the 17th Int. AMME Conference, 19-21 April, 2016
INTRODUCTION The Fe-Cu binary system is known to have low solid miscibility, and solubility is limited to only 3 %. Uenishi et. al.  and Yavari et. al.  were the first to report the formation of metastable solid solutions in the Fe-Cu system using MA technique. A wider range as well equiatomic composition have been explore and there phases formation and stability reported is depend to large extent on the different processing techniques used to produce the alloys. The majority of research concentrated on the formation of metastable phases sings to phase of Cu-Fe produced from the elemental powder blends with a positive heat of mixing. In spite the extensive studies on the system, there are many disagreement on the literature concerning the formation of single phase solid solution with homogeneous structure is possible or not [3,4] The magnetism of iron is related to its crystal structure, and it is well known, that Fe is ferromagnetic up to 1043 K when the conventional body centered cubic (bcc) structure is maintained, while Fe in face centered cubic (fcc) structure, stable at high temperature (above 1183 K), is non-magnetic . Moreover, the stabilization of Fe fcc structure, the so called -Fe, at room temperature (RT), can be achieved by substituting Fe atoms in a simple fcc lattice, such as fcc-Fe-TM those of some pure metals (Ni, Cu, Pt, Pd). When one of the immiscible Fe is ferromagnetic, the decomposition, by mechanical alloying (MA), of the supersaturated phases can allow development of low-cost new magnetic materials with large magnetoresistance and coercivities, unusually strong magnetocaloric effects, and high thermal/electrical conductivities usually unattainable in permanent magnet . The aim of this work was to study the structural transformation taking place during mechanical alloying of Cu50F50 mixture in a high energy ball mill. The produced structure of the milling were evaluated using XRD as well as scan electron microscopy. The type of the magnetic properties of the new materials was also examined.
MATERIALS AND SAMPLES Iron 99% and copper 99.9% -325 mesh powders (Alfa Asar) were placed into high energy ball milling modified attritor, rotating with 500 rpm. The powders were treated with hard steel balls at different milling times with the optimum balls to powder ratio equals to 10:1. XRD was performed using D5000 powder diffractometer using Cu K radiation
(wavelength = 0.15406 nm) with a nickel filter at 40 kV and 30 mA. The diffractometer
was operated within range of 10< 2
95 MS Proceedings of the 17th Int. AMME Conference, 19-21 April, 2016
RESULTS AND DISCUSSION X-Ray Diffraction Figure (1) presents the X-ray diffraction patterns of ball milled Cu-50wt.%Fe powder mixture. The mixture was milled for different periods up to 24 hrs. The XRD pattern of the elemental powder mixture before MM/MA shows only sharp peaks corresponding to the both metal mixture. The Fe50Cu50 samples set as a function of milling time are shown in Fig. (1). A notable intensity reductions occur as a result of severs plastic deformation after two hours milling. No additional possible new phases were detected throughout the MA process up to 7hrs.The peaks of Fe phase essentially disappear after 17 hrs milling while very broad peaks closed to (111) Cu phase developed with milling time. This implies that Cu has the lowest alloying rate among the mechanically milled elements. Moreover, disappearing of the Fe diffraction lines can be taken as indication that iron is integrated in the fccCu structure and possible given rise to the formation of solid solution phase leading to diffraction peaks shift to higher angles progressively with milling time with increasing Fe-solubility in Cu. Following mechanical milling for 12 hrs, the main peak (110) intensities of bcc Fe-phase is enhanced while fcc Cu-phase main peak (111) decreases. Such an increase of (110) - Fe peaks started after 7 hrs milling could be attributed to the relative high dislocation density reach a saturation value, and the existing dislocation rearrange and some may be annihilated. Therefore, with further milling, the lattice strain on iron peak decreases and become sharper and even the peak position may change in reverse order. On the other hand, the (111) peak continuous to further broadening and reduced in intensities which indicate a higher work hardening rate for copper compare to the second mixed element iron. Therefore, copper continuous deformed with milling with subsequent increases in lattice strain and rather the newly formed solid solution particle refinement. A 24 hours milling is needed for the powder finally transforms into very fine structure and or amorphous as a result of the accumulated energy stored produced by milling. The relative crystallinity was roughly calculated by comparing the integrated area intensity under peaks, of the MA powder with the as-received powders as a reference. From the results of the profile fitting, the relative crystallinity of the fcc Cu-phase was sharply decreased after 2hrs of MA. The bcc Fe-phase shows relative crystallinity enhancement after 7hrs of MA and then decreases to the minimum value after 17hrs. The analysis of the produced phases after different stages of milling the Cu-Fe elements powder can be in general divided into two parts.
The Formation of Nanocrystalline Supersaturated Structure The elements Fe and Cu are known to be immiscible and there is no intermediate phase exist on the equilibrium diagram. Moreover, the Cu elements are unique case where they differ only by 1.5 % in atomic radius and they are very close in electron negativity, 1.9 Cu and 1.8 Fe, with a solubility limit near 0.3 % at room temperature. To monitor the alloying process after the various stages of milling, The XRD results are examined and used to calculate the change of the d-spacing values as shown in Fig. (2).
96 MS Proceedings of the 17th Int. AMME Conference, 19-21 April, 2016
Fig. 1. X-ray diffraction patterns of mechanically milled Cu-50wt.%Fe powder at different milling time.
Fig. 2. D-values variation after mechanical alloying with different time.
97 MS Proceedings of the 17th Int. AMME Conference, 19-21 April, 2016
The results indicate that the peaks intensities reduction are associated with shift in peaks position as milling time increase and lead to a subsequent reduction of particle size of both elements, Fe and Cu. This stage of milling continuous up to 12 hrs and the observed changes could be related mainly to the increase of heterogeneous strain on the lattice of both Fe and Cu as a result of high milling energy. The continuous changes in peak profiles, broadening and displacement, are a demonstration that Fe have gradually react with Cu to form a super-saturated Cu(Fe) limited solid solution phase. The present result suggested that the fcc on lattice is expanded, with milling time up to 12 hrs, by incorporation of iron atom and resulted in an increase of the lattice parameter from 0.3615 nm to 0.3451 nm for Cu(Fe) solid solution. This result is in agreement with previously obtained values [7,8], in spite the fact that iron-atomic size is slightly larger by regard to copper. It is therefore, possible to conclude that at end of this milling stage 17 hrs, a mixture of an Cu(Fe) supersaturated phase is formed in addition to fcc (Cu) and both have a nanometer particle size. Mssboure spectroscopy analysis is also used by several authors to examine the possible local atomic alloying after milling CuFe mixtures [1, 9, and 10]. In general their results indicated that after the stages of milling up to 20 hrs, two nonmagnetic spectra are observed and attributed to the Fe(Cu) solid solution and a fcc (Fe) phase attached to the fcc (Cu) matrix. The results confirm the presence of more than one phase, but it differ in suggesting a transformation of bcc (Fe) rich in copper to an fcc (Fe) structure take place during this stage of milling. Moreover, it is important to indicate that a maximum of 3at.%Cu concentration is estimated in fcc (Fe) phase. Such transit phase is not detected up to 17 hrs of milling, where all possible Fe-peak completely disappears which could be due to the formation of a small amount of such bcc (Fe) phase